Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# TiO2 decorated functionalized halloysite nanotubes (TiO2@HNTs) and photocatalytic PVC membranes synthesis, characterization and its application in water treatment

## Abstract

In this study photocatalyst, TiO2@HNTs were prepared by  synthesizing TiO2 nanoparticles in situ on the  functionalized halloysite nanotubes (HNTs) surface. Photocatalytic PVC membrane TiO2@HNTs M2 (2 wt.%) and TiO2@HNTs M3 (3 wt.%) were also prepared. Photocatalyst TiO2@HNTs and photocatalytic PVC membranes were used to study the photocatalytic activity against the methylene blue (MB) and rhodamine B (RB) dyes in UV batch reactor. The structure and morphology of photocatalyst and photocatalytic PVC membrane were characterized by fourier transform infrared spectroscopy (FT-IR), X-ray diffraction (XRD), scanning electron microscopy (SEM), energy dispersive X-ray (EDX), transmission electron microscopy (TEM), UV-Vis spectrophotometer and photoluminescence (PL). The PL study showed that the oxygen vacancies and surface hydroxyl groups present on the surface of TiO2@HNTs act as excellent traps for charge carrier, reducing the electron-hole recombination rate.TiO2@HNTs 2 (2 wt.%) and TiO2@HNTs 3 (3 wt.%) degraded MB dye up to 83.21%, 87.47% and RB dye up to 96.84% and 96.87%, respectively. TiO2@HNT photocatalyst proved to be stable during the three consecutive cycle of photocatalytic degradation of the RB dye. TiO2@HNTs M2 and TiO2@HNTs M3 degraded MB dye up to 27.19%, 42.37% and RB dye up to 30.78%, 32.76%, respectively. Photocatalytic degradation of both the dyes followed the first-order kinetic model. Degradation product analysis was done using the liquid chromatography–mass spectrometry (LC-MS) and the results showed that the dye degradation was initiated by demethylation of the molecule. MB and RB dye degradation reaction were tested by TBA and IPA as OH* and H+ scavengers respectively. Mechanism of photocatalytic activity of TiO2@HNTs and photocatalytic PVC membrane were also explained.

## Introduction

In recent years, halloysite nanotubes (HNTs) and its composite materials have attracted enormous attention due to their wide range of potential applications in fields of catalysis1, adsorption2, composites3 and drug delivery processes4 etc. Various materials like HNTs, carbon nanotubes (CNTs), graphene oxide (GO), silica, cerium oxide5 and clay particles have been attached to photocatalysts1 to improve the photocatalytic reactions. Amongst them, HNTs (Al2Si2O5(OH)4·2H2O) is a promising material due to its efficient physicochemical property and stability which has been tested in various studies6,7,8,9. HNTs are naturally occurring, eco-friendly alumino-silicate clay minerals with tube-like structure, consisting of two-layered aluminosilicate clay mineral with one alumina octahedron sheet and one silica tetrahedron sheet in 1:1 stoichiometric ratio10,11. They are suitable for the development of photocatalyst supported materials as they enable proper distribution of composite in suspensions. The presence of HNTs improves the synergistic effects and light absorption properties of photocatalyst supported materials. Hydroxyl groups found on its surface helps in better dispersion of HNTs in different solvents12. Comparatively, HNTs are more efficient than carbon nanotubes (CNTs) due to many –OH groups present on its surface and different outside and inside chemical properties. The fact that HNTs are structurally similar to CNTs but cheaper than CNTs makes them ideal for research in photocatalysis and adsorption.

Photocatalysts are semiconductor that converts light energy into chemical energy of electron-hole pairs. An efficient photocatalyst must possess chemical and physical stability, must be cheap and nontoxic in nature13. Several semiconductor materials such as TiO2, titanate nanosheets14, cobalt hydroxide-amino complex15, ZnO16, CdS, g-C3N4 and Ag3PO4, and their nanostructure assemblies have been extensively employed as photocatalysts17.

TiO2 (nano range) has been greatly used in photocatalytic applications due to its exceptional properties such as quantum confinement and high surface to volume ratio18,19,20. Nano range TiO2 powders have large specific areas and thus provide ample active sites for reaction to occur and enhance the catalytic activity. TiO2 nanoparticles are prone to agglomerate which results in a decrease in the photocatalytic activity. Therefore, significant efforts have been made to minimize the agglomeration of TiO2 nanoparticles, such as the use of supported methods, coating technology and so on21.

HNTs as a support can also be used for nanoparticles synthesis to avoid their agglomeration11,22,23,24. TiO2 with HNTs provides large specific surface area and also due to the mesoporous structure of HNTs, they may be potentially used as adsorbents, catalysts and catalyst support25,26,27. They have also been used to efficiently remove the organic pollutants by photocatalytic degradation in aqueous dispersions28,29. TiO2 is widely used as a suitable semiconductor for treating oil spills and decomposing organic pollutants present in water and air30,31,32,33. Lvov and co-workers have extensively worked with HNTs and examined its properties by modifying it with silver nanorods, Ru, Rh, Pt, Co, Fe and copper-Nickel alloy nanoparticles to analyse the antimicrobial activity and photocatalytic activity of modified HNTs11,34,35. Papoulis et al. used anatase form of TiO2 on palygorskite and halloysite surfaces to photocatalytical decompose NOx gas under visible-light and UV light irradiation36. Du, Y. and P. Zheng calcinated the TiO2-HNT composite samples at different temperature and for TiO2-HNT calcined at 300 °C, 81.6% MB is degraded after UV irradiation treatment for 4 h37.

In another research, a one-step solvothermal method was used by Wang et al. for the preparation of TiO2/HNTs samples for wastewater purification21. Zheng et al. fabricated an amylose–HNT–TiO2 composite for effective removal of methylene blue (MB) and persistent organic pollutant 4-nitrophenol (4-NP) under UV irradiation38. Peng H. et al. fabricated the ZnO-HNTs photocatalyst and observed that ZnO bonded HNTs showed higher photocatalytic performance toward photo-degradation of MB dye9. However, it is complicated to separate nano-sized photocatalyst from treated water, and the possible toxic health effects associated with it39, hence restricting its practical application.

In some studies, nano-sized TiO2 is immobilized or dispersed onto various materials like glass40, polymer41,42 and clay43. In our previous work, we have synthesized TiO2 nanoparticles on the surface of HNTs nanocomposite via the sol-gel method and blended it in different weight percentage (1–3 wt.%) of poly(vinyl chloride) (PVC) for the preparation of hybrid ultrafiltration membranes. The new hybrid membranes had improved permeation performance and enhanced antibacterial activity against E. coli.44. Damodar et al. also observed that almost 100% of E. coli is eradicated by 4% TiO2/PVDF membrane after 1 min of UV irradiation45. Wittmer et al. prepared cellulose based TiO2 photocatalyst to treat wastewater which acts as a precursor for the preparation of catalytically active membrane. However, after the regeneration of cellulose, a partial decrease in the catalytic activity is observed46. Zhang et al. studied the rejection of Direct Black 168 by using a TiO2/Al2O3 composite membrane under UV irradiation at different pH of the wastewater. They observed that 82% of the Direct Black 168 is degraded due to TiO2/Al2O3 composite membrane under UV irradiation after 300 min47.

In this study, the HNTs surface is functionalized by using organosilane ((3-Aminopropyl)triethoxysilane)) as a coupling agent so that the HNTs surface becomes suitable for TiO2 attachment. As the raw HNTs are less adhesive in nature, there is a risk of leaching out of TiO2 during the course of the experiment. Thus the raw HNTs functionalized with organosilane coupling agent for proper attachment between TiO2 and HNTs. After functionalization of HNTs, TiO2 nanoparticles are synthesized on the surface of HNTs (TiO2@HNTs) with the help of titanium (IV) isopropoxide (TIP) and ethanol solution. Novel photocatalytic PVC membranes are prepared by blending the TiO2@HNTs photocatalyst in two different concentration i.e. 2 wt.% and 3 wt.% using a non-solvent phase induced method. The main aim for fabricating the TiO2@HNTs photocatalyst and photocatalyst membrane is to exploit the photocatalytic activity of  functionalized HNTs while avoiding the aggregation of TiO2 nanoparticles and simultaneously reducing the electron-holes recombination rate of TiO2 surface, thus improving the photocatalytic activity.

The structure and morphology of TiO2@HNTs photocatalyst and photocatalytic PVC membrane are characterized by fourier transform infrared spectroscopy (FT-IR), X-ray diffraction (XRD), scanning electron microscopy (SEM), energy dispersive X-ray (EDX), transmission electron microscopy (TEM), UV-Vis spectrophotometer and photoluminescence (PL). The photocatalytic activity of TiO2@HNTs photocatalyst (TiO2@HNTs) alone and photocatalytic PVC membranes (TiO2@HNTs M2 and TiO2@HNTs M3) are investigated by using methylene blue (MB) and rhodamine B (RB) dyes degradation test. After MB and RB dye degradation test, end products are identified by a liquid chromatography–mass spectrometry (LC-MS).

## Result and Discussions

### Characterization of TiO2@HNTs and photocatalytic PVC membranes

FT-IR spectra as shown in Fig. 1(a), confirmed the presence of functionalized HNTs after modification. When raw HNTs48 were compared with the TiO2@HNTs, some new FTIR peaks were observed in the spectrum like stretching CH2 vibration band around 2934 cm−1, and the deformation CH2 and Si-CH vibration at 1627 cm−1 and1507 cm−1 respectively. Apart from these peaks, broad peak of O-H stretching of water at 3433 cm−1 was also seen. These observations confirmed the presence of silane coupling agent49. Silane coupling agent is used because its main function is to ensure proper bonding between TiO2 and HNTs49,50,51,52. If this functionalization is not done, due to the absence of chemical conjugation53, the TiO2 may leach out during the course of the experiment because of the less adhesive nature of raw HNTs54,55. The TiO2@HNTs possess some significant signals, like distortions of aluminium-oxygen-silicon and silicon-oxygen-silicon bonds at 538 and 468 cm−1 respectively; and -OH groups of the inner hydroxyl groups at 909 cm−1. Furthermore, for comparison, the broad stretching band of silicon-oxygen at about 1037 cm−1 shifts to about 1058 cm−1, indicating hydrogen bonding between TiO2 and HNTs21. In Fig. 1(b), ATR-FT-IR spectra of TiO2@HNTs M0 and TiO2@HNTs M3 with the principle bands of PVC were depicted. FT-IR spectrum of PVC reflects expected distinctive absorptions: 2970–2912 cm−1 attributed to stretching C-H of CHCl and stretching C-H of CH2 group, 1435 cm−1 and 1427 cm−1 attributed to deformation wagging of CH2 group, and 1331–1255 cm−1 shows the stretching of the C-H of CHCl groups. Stretching C-C (1092 cm−1), rocking CH2 (811 cm−1), stretching C-Cl attributed to 688 cm−1 and 618 cm−1 respectively56. In Fig. 1b, the peaks of photocatalyst PVC membrane in the ATR-FT-IR results resembles the characteristic peaks belonging to both TiO2@HNTs M0 and TiO2@HNTs M3. Other characteristic absorption peaks for TiO2@HNTs in the spectrum of the membrane was not clearly identified because of the overlap with absorption peaks of PVC polymer or the IR beam might not be able to penetrate properly enough to get distinct peaks of HNTs57 in FTIR spectra (Fig. 1b).

The results of XRD clearly shows the specific peaks as shown in Fig. 1(c) which compares the XRD results of HNTs and TiO2@HNTs synthesized. The peaks depicted for HNT sample can be translated into the characteristic peaks of halloysite shown in Fig. 1(c). Two fresh peaks, however, can be noticed at 2θ = 48° and 54.1° and a stronger peak at 2θ = 25.3° alongside with decline in the halloysite peaks due to the sol-gel method. Based on JCPDS 21–1272, all peaks related to TiO2 properties can be indexed to the (101), (004), (200) and (105) planes of TiO2 structure58,59. This verifies the successful preparation of TiO2@HNTs. Similar results of XRD pattern also described by the Ghanbari et al., in their study for the fabrication of high-performance thin film nanocomposite membranes60. Furthermore, in the EDX spectrum (Fig. 1d) confirms the loading of TiO2 nanoparticles on the surface of HNTs with 24.42 wt%. Intense peaks of Ti and oxygen at 0.5 eV were observed which confirmed the presence of TiO2 nanoparticles on the surface of HNTs.

Thermal behaviour of TiO2@HNTs and TiO2@HNTs/PVC blends was investigated from room temperature to 600 °C temperature range. The temperature was raised at the rate of 10 °C/min (Fig. 2). The raw HNTs showed a weight loss between 50 °C and 150 °C, which may be due to reduction in adsorbed water molecules61; and structural dehydroxylation of structural Al–OH groups between 450–550 °C62. Decomposition of the (3-Aminopropyl) triethoxysilane causes an additional weight loss in TiO2@HNTs between 250 °C and 425 °C when compared with the raw HNTs63 suggesting that the thermal stability, as well as the purity of the nanotubes, was high. PVC membrane (TiO2@HNTs M0–0 wt.%) and TiO2@HNTs membranes (TiO2@HNTs M2 and TiO2@HNTs M3) showed a different behaviour. The weight loss of the sample (around 60%) was mainly between temperature range 220 °C to 300 °C. The rest of the sample was thermally decomposed at 500 °C as shown in Fig. 2

FEG-SEM and TEM were done to analyse the structural and morphological characteristics of raw HNTs and TiO2@HNTs photocatalyst (Fig. 3). The TEM images of raw HNTs clearly show the hollow tubular structure with a diameter of 50–70 nm and length of 0.5–2 µm (Fig. 3c). The outer surface of HNTs was made up of silica and was surrounded by multi-walled aluminol layer. In Fig. 3b,d TiO2 nanoparticles were seen to be randomly deposited on the surface of HNTs. Few aggregation or cluster of nanoparticles was observed in FEG-SEM and TEM analysis (Fig. 3b,d) which was formed when photocatalyst was separated from the solution during the fabrication process. The size of small particles and cluster size of this TiO2 range from 10 nm to 80 nm. The presence of TiO2 nanoparticles on the surface of HNTs confirms successful loading on HNTs.

All the membrane possessed typical asymmetric structure like that of ultrafiltration membranes and no distinct difference between the TiO2@HNTs M0 (Fig. 4a) and the TiO2@HNTs M2 and TiO2@HNTs M3 (Fig. 4b,c) on the top surface was observed. Only large pores were observed on the membrane surface as shown in Fig. 4(b,c) when compared with TiO2@HNTs M0 (Fig. 4a). FEG-SEM images shows top surface and cross-sectional view of TiO2@HNTs M0 and TiO2@HNTs M2 and TiO2@HNTs M3 membranes. All membrane samples were homogeneous and asymmetric in nature with macro-voids and finger-like structures formed because of the high mutual diffusivity of DMAc and water. This porous structure indicates that TiO2@HNTs increases the membrane porosity without altering the membrane morphological structure64.

To investigate the recombination of the free carrier in HNTs, photoluminescence (PL) emission spectrum was analysed. One broad PL peak centred under excitation of 450 nm visible light irradiation was observed in Fig. 5a. The broad-band at 624 nm indicates that the light for excitation can initiate electron transition from the valence band (VB) to the conduction band (CB) in HNTs. As a result of this transition, the electron/hole pair can be generated which then further recombine radiatively to give broad and strong PL signal under 450 nm light irradiation. The PL emission spectrum of TiO2@HNTs was recorded at an excitation wavelength of 220 nm (high absorption region). The major peak at 361 nm (lower than the band edge emission) in PL emission spectra (Fig. 5b) was due to the band to band transition. At longer wavelengths in the visible region, the emission peaks at 421, 445, 481, 535 and 556 nm reflect the surface state emissions, located within the band gap of TiO2@HNTs65. The oxygen vacancies and surface hydroxyl groups present on the surface of TiO2 and HNTs acts as excellent traps for charge carrier, reducing the electron-hole recombination rate. Presence of oxygen vacancies from shallow trap state near the adsorption band edge act as efficient electron trap centres or colour centres. UV-Vis spectroscopy was used to study the light absorption properties. Figure 5c displays the UV-Vis absorption spectra of the prepared materials obtained. The band gap of pure TiO2 is 3.2 eV and the absorption edge of the TiO2@HNTs material is around 220 nm corresponding to the band gap energy (Eg) of 3.66 eV (Fig. 5d). This difference is due to the addition of HNTs because of which the modified photocatalyst gets excited to produce more electron-hole pairs under light irradiation, resulting in higher photocatalytic activity66,67.

### Photocatalytic activities of TiO2@HNTs photocatalyst and photocatalytic PVC membranes for the degradation of MB and RB dye solutions

In Fig. 6 images of MB and RB dye degradation under 120 min of UV irradiation can be seen. Initially, the colour of MB dye solution was blue and RB dye solution was pink. After 120 min, the colour of TiO2@HNTs 2 and 3 reaction mixture changed from blue to light blue in case of MB dye and from pink to colourless solution in case of RB dye.

This decolourization was due to degradation of dye and was highest in the case of TiO2@HNTs 3. The chemical structure of MB and RB dye is shown in Fig. 7(a,b). To further confirm the degradation of dye, LC-MS chromatographic separation analysis was done. For the analysis, the dye solution was collected after 120 min of UV irradiation. As seen in Fig. 8(a–d), maximum absorption of MB dye in the visible region was at 664 nm and in the UV region two peaks located at 245 and 292 nm. The highest peak of MB dye at 664 nm is due to its centre benzene ring comprising sulphur and nitrogen whereas the two dimethylamine substituted aromatic ring exhibits its peak in the UV region at 245 and 292 nm. These high peaks at 664 nm gradually diminish with time in the presence of TiO2@HNTs 3 under UV irradiation. Similarly, for RB dye, the characteristic absorption peak at 554 nm as shown in Fig. 9(a–d) also degrades with time. The n → π transition of C=N, C=O groups in the aromatic ring of the RB dye structure (Fig. 7b) is responsible for the colour of solution and its absorbance at 554 nm. During the reaction process, when the dye structure was disrupted by the TiO2@HNTs 3 photocatalyst, the absorption intensity of RB dye decreased rapidly with change in colour from pink to a colourless solution.

Though photocatalytic PVC membranes TiO2@HNTs M2 and TiO2@HNTs M3 both exhibited photocatalytic activity (as shown in Figs 8c,d and 9c,d for MB and RB dyes respectively), but TiO2@HNTs M3 membrane possessed more catalytic activity as compared to TiO2@HNTs M2 because with the increase in the TiO2@HNTs concentration the catalytic activity also enhances. However, it was observed that photocatalytic activity reduced in photocatalytic PVC membranes when compared with the same wt% of TiO2@HNTs alone. The MB dye was degraded up to 27.19%, 42.37% (Fig. 8c,d) and RB upto 30.78%, 32.76% (Fig. 9c,d) for TiO2@HNTs M2 and TiO2@HNTs M3 respectively. The reason behind this slow rate of degradation in both TiO2@HNTs M2 and TiO2@HNTs M3 can be due to the reduction of active sites of TiO2@HNTs photocatalyst during membrane preparation. During phase separation process, the increase in the amount of TiO2@HNTs photocatalyst increases its catalytic activity but its increase after 3 wt.% in membrane casting solution may result in photocatalyst agglomeration69. This agglomeration hampers the number of free catalytic sites for dye degradation and also delays the phase separation process during membrane preparation46. When the concentration of photocatalyst increases in the solution, the turbidity of the solution increases and light is scattered more due to which screening effect occurs hampering the specific activity of the catalyst and reducing the degradation rate70,71,72. Thus an optimal amount of photocatalyst must be used for photocatalytic degradation process for increased degradation and reduced inaccuracy.

The kinetics of photocatalytic reactions can be described using the first-order reaction for concentrations (20 mg/L) of MB and RB dye solutions. The rate constants (k) and the correlation coefficient (R2) has been evaluated using linear regression curve of ln(C0/C) versus UV light irradiation time. First-order rate equations are as follows73:

$$\mathrm{ln}\,\frac{[{C}_{0}]}{[C]}={\rm{kt}}$$
(1)

Here, k is the first order rate constant (min−1); [C] and [C0] final and initial dye concentration in (mg/L), respectively.

The degradation efficiency has been calculated using74:

$${\rm{Degradation}}( \% )=(\frac{{C}_{0}-C}{{C}_{0}})\times 100$$
(2)

where C0 is the initial concentration of the dye and C is the concentration of the dyes after UV irradiation in the selected time interval.

The correlation coefficient (R2) was calculated to be nearly as high as R2 ≈ 0.95–0.99 which reiterate the suitability of the first-order reaction listed in Table 1. MB and RB degradation rate are shown in Fig. 10c,d, where the TiO2@HNTs photocatalyst has notably improved the photocatalytic activity. During photocatalysis of RB dye by TiO2@HNTs 2 and 3, dye adsorption process occurred in two steps shown in Fig. 10d. At first stage, RB molecules diffuse from the aqueous solution to the external surface of TiO2@HNTs or the boundary layer diffusion of RB molecules. Secondly, gradual adsorption occurred until equilibrium was reached. The linear portion of the first stage did not pass through the origin, indicating the existence of a boundary layer resistance between TiO2@HNTs photocatalyst and dye solution75 Similar observation is reported in literature73. Furthermore, the detailed photocatalytic mechanism is described in detail in a later section.

The stability of the TiO2@HNTs photocatalyst was estimated by recycling the photocatalyst for degradation of RB dye under UV light irradiation for three times. The loss of the photocatalytic activity was negligible (approximately 6% after 3 repeated runs) (Fig. 11) which signifies the stability of TiO2@HNTs photocatalyst in terms of its non photo-corrosive nature during the photocatalytic degradation of the model dye molecules, which proved to be very important for its practical applications.

### Photocatalytic PVC membrane activity Test with MB dye

To evaluate the photocatalytic property of the membrane surface, control (raw PVC membrane TiO2@HNTs M0), TiO2@HNTs M2 and TiO2@HNTs M3 samples were treated with UV light without stirring for 1 h (Fig. 12). After 1 h of irradiation TiO2@HNTs M2 and TiO2@HNTs M3, sample colour disappears from the membrane surface. On the contrary, the change in colour in control experiment was less after irradiation of UV light. The change in colour of membrane of the control sample was seen to be least when irradiated with UV light, which was contrary to the result of samples of TiO2@HNTs M2 and TiO2@HNTs M3. TiO2 acts as a semiconductor and presence of UV light results in the formation of electrons and holes. These photo-generated electrons hence formed, reduces Ti (IV) cations to the Ti (III) state and the holes oxidise O2* anions76. Simultaneously O2 atoms are propelled out producing a set of O2 vacancies on the surface. These vacancies were filled by water molecules present in the environment and adsorbed OH groups are formed on the surface, increasing the hydrophilicity of the surface77. Also, the radicals hence produced can degrade the dye molecules present around the membrane surface (detail mechanism explained in the mechanism section). For the reproducibility, a test procedure was repeated with five membrane pieces for each sample. MB dye showed better contrast while taking digital images and hence was preferred for photographic images.

### Photocatalytic Mechanism of TiO2@HNTs photocatalyst and Photocatalytic membrane

When irradiated with UV light, the HNTs do not get excited, rather it acts as an electrical insulator and hence any charge generated on TiO2 surface during UV irradiation cannot be transferred to HNTs. These electrostatic attraction and repulsion forces contribute together for an efficient movement and separation of e and h+ on TiO21. Apart from being a charge carrier separator, HNTs also enhance dye degradation. Due to the negatively charged surface of HNTs, the dye molecule (cationic in nature) are brought closer to the TiO2, increasing the adsorption rate of the dye molecules. The detailed mechanism of the photocatalyst TiO2@HNTs and photocatalyst membrane are shown in Fig. 13. When TiO2@HNTs is irradiated by UV light, a photoelectron moves from valence band of TiO2@HNTs to the empty conduction band. This photon has the energy (hυ) equal to or greater than the band gap. Thus a hole is created in VB ($${{\rm{h}}}_{{\rm{VB}}}^{+}$$) and an electron ($${{\rm{e}}}_{{\rm{CB}}}^{-}$$) in CB generated as shown in Fig. 13(a).These ($${{\rm{h}}}_{{\rm{VB}}}^{+}$$) then produce OH* radical after reacting with H2O. Now, these OH* radicals act as a potent oxidising agent and oxidise adsorbed organic molecules which are in near vicinity of TiO2@HNTs surface Fig. 13b. Simultaneously O2 atoms are propelled out producing a set of O2 vacancies on the surface. These vacancies are filled by water molecules present in the environment and results in the formation of adsorbed OH groups on the surface, increasing surface hydrophilicity77. These photo-generated electrons hence formed, reduces Ti+4@HNTs cations to the Ti+3@HNTs state and the holes oxidise O2* anions. Also, the radicals hence produced can degrade the dye molecules present around the membrane surface as shown in Fig. 13c. The efficiency of the breakdown of these organic molecules depends upon their stability and structure. OH* radicals also degrade the pollutant present around it. The electrons in ($${{\rm{e}}}_{{\rm{CB}}}^{-}$$) conduction band meanwhile reacts with O2 and generate superoxide radicals (O2*), which accelerates oxidation process (Fig. 13d) and also hinders any further e−/hole recombination formation, thus maintaining electron neutrality within the TiO2 molecule. The H+ formed in reaction further reacts with O2* formed and protonates the hydroperoxyl radical (HO2*). Hence finally hydroxyl radical (OH*) is formed, which is highly reactive in nature.

The experimental data confirm that after 120 min of UV irradiation, the dye solution gets degraded with the formation of intermediate and end products. A mass spectroscopic (MS) study of the dye solution was also done to determine the intermediate and end products which were formed due to the cleavage of aromatic rings during the dye degradation process and eluted out at different retention time as per their mass and suggested structures. The difference in the concentration and composition of the products lead to many peaks with different intensities. Mass spectra and the possible structures of the dye degradation products are listed in Supplementary Table S2 and Table S3 for MB and RB dye79,80,81. The demethylation cleavage has also been reported in the literature during the photocatalytic degradation79,80,82,83,84.

For evaluation of the activity of a photocatalyst, commonly time dependence of the concentration loss of dye under UV irradiation is measured. However, there are many factors that govern the reaction rate and kinetics. These experimental conditions include the concentration of the photocatalyst, the surface area of the photocatalyst, the amount of the photocatalyst used in the experiment and the UV light intensity and more. Table 2 summarises some recently synthesized photocatalyst with their photocatalytic experimental data.

## Conclusion

Utilization of naturally present HNTs as photocatalyst support is advantageous for the synthesis of TiO2@HNTs photocatalyst nanoparticles due to its size and shape dependent photocatalytic properties. In this study, TiO2@HNTs photocatalyst and photocatalytic PVC membranes are  synthesized. The prepared photocatalyst is stable and exhibits enhanced photocatalytic activity for the degradation of MB and RB dye solution under UV irradiation. The photocatalytic PVC membrane also exhibits similar photocatalytic activity against MB and RB dye but the degradation is slower as compared to the TiO2@HNTs photocatalyst of the same weight.

Due to the electrostatic interaction between TiO2 and HNTs surface, the photocatalyst has more e and h+ pairs resulting in high photocatalytic activity. In the case of MB and RB dye which are positively charged, HNTs improved the supply and stability of the photo-generated charges and enhanced the absorption capability of the dye molecule on the photocatalyst. This was because of electrostatic attractive and repulsion forces originating from the negatively charged HNTs surface. The stability of the TiO2@HNTs photocatalyst is non photo-corrosive nature during the three consecutive cycle of photocatalytic degradation of the model dye molecules, which is very important for its practical applications. The MB and RB degradation catalysed by a TiO2@HNTs and photocatalyst PVC membrane followed the first-order kinetic model. Therefore, the capabilities of nano range TiO2@HNTs photocatalyst to degrade dyes may be exploited for wastewater purification in various textile and chemical industries.

## Materials and Methods

### Materials

HNTs, Titanium (IV) isopropoxide(TTIP) and Poly (vinyl chloride) polymer were furnished by Sigma-Aldrich. (3-Aminopropyl)triethoxysilane (silane coupling agent) was purchased from Himedia. Tert-butyl alcohol (TBA) (99%) and isopropanol (IPA) (99%) were purchased from s-d Fine Chem. Ltd, Mumbai. Rhodamine B (RB) and Methylene blue (MB) dyes were provided by Colourtex Pvt. Ltd., Surat, Gujarat. All other chemicals were also of analytical grade and were used without any purification. The water used was Elix millipore pure water (DI).

#### TiO2@HNTs photocatalyst preparation

For the preparation of photocatalyst, moisture was removed from the inner/outer surfaces of raw HNTs by drying them for 4 h at 400 °C. 30 ml of silane coupling agent was mixed with 100 ml of toluene and 10 g of dried HNTs was then added into the silane-toluene solution to make it functional53. The mixture was then stirred at 125 °C for 18 h. After this, the mixture of functionalized HNTs was centrifuged and then washed with isopropanol (3–4 times). Vacuum drying chamber was further used for drying of the pellet at 60 °C. To synthesize TiO2 nanoparticles on functionalized HNTs surface, 1 g of silane HNTs was mixed with titanium (IV) isopropoxide (TIP) - ethanol solution (ratio 1:15) by dispersing it into the deionised water (pH value adjusted by adding HNO3 or NH4OH). This solution was then vigorously stirred for sol-gel preparation. Hydrolysis reaction was initiated when TIP solution interacted with water molecules making the solution turbid and resulting in the increase of temperature to 60–70 °C for 18–20 h. When the peptization process was complete, stirring was stopped and centrifugation was done to retrieve TiO2@HNTs mixture, which was then subjected to vacuum drying chamber overnight at 65 °C85,86. At last, the calcination of TiO2@HNTs was done by heating it in a muffle furnace for 2 h (400 °C)44.

#### Photocatalytic PVC membranes

The photocatalytic PVC membranes were prepared based on the principle of classical phase inversion method. The mixture containing TiO2@HNTs photocatalyst (2 wt.% and 3 wt.% by weight of PVC) and DMAc solvent (85 wt.% by weight of the solution) was stirred at 600 rpm for 1 h to get the photocatalyst dispersed properly in the solvent. For the formation of pores, PVP (1 wt.% by weight of the solution) and PVC (14 wt.% by weight of the solution) polymer were added into the mixture (shown in Table 3). For uniform dispersion, the mixture was vigorously stirred for 12 h. After stirring, a homogeneous casting solution thus obtained was then degassed (room temperature) and poured on a glass slide with the help of membrane applicator (thickness 150 µm). The glass plate was then dipped immediately in a pure water bath for 12 h (room temperature) for the proper phase inversion process. Two photocatalytic PVC membranes (Table S4) were prepared based on the weight% of TiO2@HNTs photocatalyst added in the membrane casting solution.

### Characterizations

#### Fourier transform-infrared (FT-IR) spectroscopy

3000 Hyperion Microscope with Vertex 80 FTIR System (Bruker, Germany) was used for the characterization of raw HNTs, TiO2@HNTs and photocatalytic membrane. Scan range was 450–4500 cm−1.

#### Thermo-gravimetric analysis (TGA)

Samples were heated from room temperature to 600 °C at the rate of 10 °C min−1 under flowing nitrogen using a Diamond TG/DTA (Perkin Elmer, USA) instrument.

#### X-ray diffraction (XRD)

HNTs and TiO2@HNTs Photocatalyst powder samples were put into the sample collector for X-ray diffraction analysis with PANalytical, The Netherlands, scan rate 2 degrees/min. XRD peaks were recorded in the reflection mode in the angular range of 10–80° with (2 theta) angle.

#### Transmission electron microscopy (TEM)

The morphological characteristics of raw HNT and TiO2@HNTs were studied by a CM 200 transmission electron microscope (Philips). The samples were dispersed in deionized water, and then the suspended particles were transferred to a copper grid.

#### Field emission gun-scanning electron microscopes (FEG-SEM) with EDS

JSM-7600F FEG-SEM was used for determination of the structure of raw HNT and TiO2@HNTs which had an energy dispersive X-ray spectrum (EDS, Inca Energy-200) at an accelerating voltage of 200 kV.

#### Photoluminescence spectra

At room temperature, the photoluminescence spectra were recorded with a Cary Eclipse fluorospectrometer using 220 and 450 nm Ar+ laser as excitation source.

#### Band gap energy

For determining the absorption coefficient, optical energy gap (Eg) and nature of transitions involved, the optical absorbance spectra of TiO2@HNTs (at room temperature) were studied. The thickness of the quartz cuvette (t), the optical absorption coefficient (α) was determined from the measurement of wavelength (λ). Generally,the absorption coefficient (α) was related to photon energy (hν) by known equation87,88:

$$({\rm{\alpha }}{\rm{h}}{\rm{\nu }})={\rm{\beta }}({\rm{h}}{\rm{\nu }}-{{\rm{E}}}_{{\rm{g}}}{)}^{{\rm{n}}}$$

where, β signifies a constant known as band tailing parameter, Eg: energy of the optical band gap and n: power of the transition.

To convert the absorption spectra, in place of α, the kubelka-Munk function was used to eliminate any tailing contribution from UV spectra. The following function was applied to convert the absorption spectra:

$$F(R)=\frac{{(1-R)}^{2}}{2R}$$

where R, the reflectance Eg values were estimated from plot of (F(R) hν)2 versus energy by extrapolating the linear part.

#### Liquid chromatography–mass spectrometry (LC-MS)

The chromatographic experiments with LCMS system were carried out on an Agilent 1290 Infinity UHPLC System, 1260 infinity Nano HPLC with Chipcube, 6550 iFunnel Q-TOFs (Agilent Technologies, USA) with a Column, binary pump and an autosampler. Acetonitrile was used as mobile phase solvent. The mass spectrometer was equipped with an electrospray ionization (ESI) source. The mass range was from 50 to 1000 m/z. Degradation products were monitored by LC-MS. Measurement conditions are listed in Supplementary Table S1.

### Methods

#### Photo-catalytic reaction experiments

The possible photocatalytic activities of the TiO2@HNTs 2, TiO2@HNTs 3, TiO2@HNTs M2 and TiO2@HNTs M3 membranes were examined by assessing the MB and RB dye degradation which was prepared in an aqueous medium. UV batch reactor was used to carry out the photocatalytic reaction at a low pressure of 125 W UV lamp (254 nm) and Photon flux (Φ) = 1.69 × 1020 s−1 m−2 with continuous stirring. The photoreactor was initially filled with 100 mL of a 20 mg/L aqueous dye solution along with different weight percentage of a photocatalyst for the process and also with a different weight percentage of photocatalytic PVC membranes. The different concentration and combination used in the reactorare mentioned below. A UV−visible spectrophotometer (HACH, DR 6000, USA) was used to record the absorption magnitude of the dye solution regularly and similar steps was performed for both the dyes, after regular time intervals, at wavelengths of 664 nm for MB and 562 nm for RB dye respectively. Similarly, the photocatalytic efficiency of photocatalytic PVC membranes (TiO2@HNTs M2 and TiO2@HNTs M3) were also assessed. Initially, the membranes were dried and cut into small pieces and then dispersed into the aqueous dye solution for 1 h under constant stirring, after which dye solution irradiated with UV light, the concentration was analysed by a UV−visible spectrophotometer at regular intervals.

For comparative analysis, two different weight percentage of TiO2@HNTs photocatalyst (accordingly photocatalyst added in membrane casting solution) and photocatalytic PVC membranes were used for this study under following conditions –

1. (i)

MB and RB dye solution exposed to UV light in the absence of HNTs, TiO2@HNTs photocatalyst and photocatalytic PVC membrane (adsorption of dyes).

2. (ii)

MB and RB dye solution irradiated with UV light with only HNTs. (denoted as HNTs 2 and HNTs 3 i.e 2 wt.% and 3 wt.%)

3. (iii)

MB and RB dye solution were irradiated with UV light with only TiO2@HNTs photocatalyst (denoted as TiO2@HNTs 2 and TiO2@HNTs 3, a similar weight of photocatalyst added in membrane casting solution). In addition, we have also taken a higher concentration of photocatalyst in the reaction.

4. (iv)

MB and RB dye solution irradiated with UV light with photocatalytic PVC membranes (denoted as TiO2@HNTs M2 and TiO2@HNTs M3 i.e 2 wt.% and 3 wt.% photocatalyst added in membrane casting solution as mentioned in membrane preparation section)

5. (v)

Scavenger effects on the MB and RB dye degradation reaction were also tested by using TBA and IPA (with 0.2 mmol solutions) as hydroxyl radical (OH*) and H+ scavengers respectively.

Adsorption experiments were performed containing 2 wt.% and 3 wt.% of TiO2@HNTs photocatalyst and dye solution (20 mg/L MB and RB). The conical flasks were placed on a magnetic stirrer for 2 h. MB and RB dye concentrations in the solution were analyzed by UV-Vis spectrophotometer at different time intervals during the reaction. The amount of dye on TiO2@HNTs photocatalyst adsorb was calculated from the following equation

$${q}_{e}=\frac{({c}_{i}-{c}_{f})\times V}{M}$$

where, qe (mg/g): the amount of dye adsorbed, Ci and Cf (mg/L): the concentrations of dye at initial and equilibrium respectively, V (L): the volume of the solution and M (g): the mass of dry TiO2@HNTs photocatalyst used.

#### Photocatalytic PVC membrane activity test with MB dye

Photocatalytic PVC membrane TiO2@HNTs M2 and TiO2@HNTs M3 pieces (1 cm2 per piece) with control membrane were dipped into 20 ml aqueous dye solution of MB dye and kept in dark for1 h. Membrane pieces were then positioned in open petri dishes individually and kept in UV light (Philips 15 W UV light). Digital images of these membranes were captured after keeping them on petri plates in dark and after exposure to UV light.

## References

1. 1.

Christoforidis, K. et al. Solar and visible light photocatalytic enhancement of halloysite nanotubes/gC 3 N 4 heteroarchitectures. RSC Advances 6, 86617–86626 (2016).

2. 2.

Cavallaro, G., Lazzara, G., Milioto, S., Parisi, F. & Sanzillo, V. Modified halloysite nanotubes: nanoarchitectures for enhancing the capture of oils from vapor and liquid phases. Applied Materials & Interfaces 6, 606–612 (2013).

3. 3.

Amjadi, M., Samadi, A. & Manzoori, J. L. A composite prepared from halloysite nanotubes and magnetite (Fe3O4) as a new magnetic sorbent for the preconcentration of cadmium(II) prior to its determination by flame atomic absorption spectrometry. Microchimica Acta 182, 1627–1633, https://doi.org/10.1007/s00604-015-1491-y (2015).

4. 4.

Sun, P. et al. Effective activation of halloysite nanotubes by piranha solution for amine modification via silane coupling chemistry. RSC Advances 5, 52916–52925 (2015).

5. 5.

Lakhotia, S. R., Mukhopadhyay, M. & Kumari, P. Cerium oxide nanoparticles embedded thin-film nanocomposite nanofiltration membrane for water treatment. Scientific reports 8, 4976 (2018).

6. 6.

Zhai, R. et al. Immobilization of enzyme biocatalyst on natural halloysite nanotubes. Catalysis Communications 12, 259–263 (2010).

7. 7.

Zhang, Y., Ouyang, J. & Yang, H. Metal oxide nanoparticles deposited onto carbon-coated halloysite nanotubes. Applied Clay Science 95, 252–259 (2014).

8. 8.

Lvov, Y. M., Shchukin, D. G., Mohwald, H. & Price, R. R. Halloysite clay nanotubes for controlled release of protective agents. ACS nano 2, 814–820 (2008).

9. 9.

Peng, H., Liu, X., Tang, W. & Ma, R. Facile synthesis and characterization of ZnO nanoparticles grown on halloysite nanotubes for enhanced photocatalytic properties. Scientific reports 7, 2250 (2017).

10. 10.

Ballav, N., Choi, H. J., Mishra, S. B. & Maity, A. Polypyrrole-coated halloysite nanotube clay nanocomposite: synthesis, characterization and Cr (VI) adsorption behaviour. Applied Clay Science 102, 60–70 (2014).

11. 11.

Vinokurov, V. A. et al. Formation of metal clusters in halloysite clay nanotubes. Science and Technology of advanced MaTerialS 18, 147–151 (2017).

12. 12.

Zhang, Y., Tang, A., Yang, H. & Ouyang, J. Applications and interfaces of halloysite nanocomposites. Applied Clay Science 119, 8–17 (2016).

13. 13.

Molinari, R., Caruso, A. & Palmisano, L. In Comprehensive Membrane Science and Engineering (eds Enrico Drioli & Lidietta Giorno) 165–193 (Elsevier, 2010).

14. 14.

Soontornchaiyakul, W., Fujimura, T. & Sasai, R. Photocatalytic Oxidative Decomposition of Methylene Blue by Rh-Doped Titanate Nanosheets ([Ti4− x Rh x O9] 2−). Bulletin of the Chemical Society of Japan 90, 1267–1272 (2017).

15. 15.

Walsh, D., Sanchez-Ballester, N. M., Ting, V. P., Ariga, K. & Weller, M. T. Visible light promoted photocatalytic water oxidation: proton and electron collection via a reversible redox dye mediator. Catalysis Science &. Technology 6, 3718–3722 (2016).

16. 16.

Maeda, K. & Domen, K. Development of novel photocatalyst and cocatalyst materials for water splitting under visible light. Bulletin of the Chemical Society of Japan 89, 627–648 (2016).

17. 17.

Wen, J., Xie, J., Chen, X. & Li, X. A review on g-C3N4-based photocatalysts. Applied surface science 391, 72–123 (2017).

18. 18.

Lakhotia, S. R., Mukhopadhyay, M. & Kumari, P. Surface-modified nanocomposite membranes. Separation & Purification Reviews, 1–18 (2017).

19. 19.

Yu, J., Liu, W. & Yu, H. A one-pot approach to hierarchically nanoporous titania hollow microspheres with high photocatalytic activity. Crystal growth and design 8, 930–934 (2008).

20. 20.

Nguyen-Phan, T.-D., Kim, E. J., Hahn, S. H., Kim, W.-J. & Shin, E. W. Synthesis of hierarchical rose bridal bouquet-and humming-top-like TiO2 nanostructures and their shape-dependent degradation efficiency of dye. Journal of colloid and interface science 356, 138–144 (2011).

21. 21.

Wang, R. et al. Photocatalytic activity of heterostructures based on TiO2 and halloysite nanotubes. ACS applied materials & interfaces 3, 4154–4158 (2011).

22. 22.

Jiang, G., Lin, Z., Zhu, L., Ding, Y. & Tang, H. Preparation and photoelectrocatalytic properties of titania/carbon nanotube composite films. Carbon 48, 3369–3375 (2010).

23. 23.

Wang, S., Wang, T., Chen, W. & Hori, T. Phase-selectivity photocatalysis: a new approach in organic pollutants’ photodecomposition by nanovoid core (TiO2)/shell (SiO2) nanoparticles. Chemical Communications, 3756–3758 (2008).

24. 24.

Zou, W., Zhang, J. & Chen, F. Preparation, characterization and application of TiO 2 nanoparticles surface-modified by DDAT. Materials Letters 64, 1710–1712 (2010).

25. 25.

Occelli, M. L. New routes to the preparation of pillared montmorillonite catalysts. Journal of Molecular Catalysis 35, 377–389 (1986).

26. 26.

Sterte, J. Synthesis and properties of titanium oxide cross-linked montmorillonite. Clays and Clay Minerals 34, 658–664 (1986).

27. 27.

Ménesi, J. et al. Photocatalytic oxidation of organic pollutants on titania–clay composites. Chemosphere 70, 538–542 (2008).

28. 28.

Kibanova, D., Trejo, M., Destaillats, H. & Cervini-Silva, J. Synthesis of hectorite–TiO2 and kaolinite–TiO2 nanocomposites with photocatalytic activity for the degradation of model air pollutants. Applied Clay Science 42, 563–568 (2009).

29. 29.

Mogyorósi, K., Farkas, A., Dékány, I., Ilisz, I. & Dombi, A. TiO2-based photocatalytic degradation of 2-chlorophenol adsorbed on hydrophobic clay. Environmental science & technology 36, 3618–3624 (2002).

30. 30.

Nishimoto, S.-I., Ohtani, B., Kajiwara, H. & Kagiya, T. Correlation of the crystal structure of titanium dioxide prepared from titanium tetra-2-propoxide with the photocatalytic activity for redox reactions in aqueous propan-2-ol and silver salt solutions. Journal of the Chemical Society, Faraday Transactions 1: Physical Chemistry in Condensed Phases 81, 61–68 (1985).

31. 31.

Hoffmann, M. R., Martin, S. T., Choi, W. & Bahnemann, D. W. Environmental applications of semiconductor photocatalysis. Chemical reviews 95, 69–96 (1995).

32. 32.

Martı́, M., Fetter, G., Domı́, J., Melo-Banda, J. & Ramos-Gomez, R. Catalytic hydrotreating of heavy vacuum gas oil on Al-and Ti-pillared clays prepared by conventional and microwave irradiation methods. Microporous and Mesoporous Materials 58, 73–80 (2003).

33. 33.

El-Kemary, M., Abdel-Moneam, Y., Madkour, M. & El-Mehasseb, I. Enhanced photocatalytic degradation of Safranin-O by heterogeneous nanoparticles for environmental applications. Journal of Luminescence 131, 570–576 (2011).

34. 34.

Sanchez-Ballester, N. M. et al. Activated interiors of clay nanotubes for agglomeration-tolerant automotive exhaust remediation. Journal of Materials Chemistry A 3, 6614–6619 (2015).

35. 35.

Abdullayev, E. et al. Natural tubule clay template synthesis of silver nanorods for antibacterial composite coating. ACS applied materials & interfaces 3, 4040–4046 (2011).

36. 36.

Papoulis, D. et al. Palygorskite-and halloysite-TiO2 nanocomposites: synthesis and photocatalytic activity. Applied Clay Science 50, 118–124 (2010).

37. 37.

Du, Y. & Zheng, P. Adsorption and photodegradation of methylene blue on TiO2-halloysite adsorbents. Korean Journal of Chemical Engineering 31, 2051–2056 (2014).

38. 38.

Zheng, P., Du, Y., Chang, P. R. & Ma, X. Amylose–halloysite–TiO2 composites: preparation, characterization and photodegradation. Applied surface science 329, 256–261 (2015).

39. 39.

Gwinn, M. R. & Vallyathan, V. Nanoparticles: health effects—pros and cons. Environmental health perspectives 114, 1818 (2006).

40. 40.

Hofstadler, K., Bauer, R., Novalic, S. & Heisler, G. New reactor design for photocatalytic wastewater treatment with TiO2 immobilized on fused-silica glass fibers: photomineralization of 4-chlorophenol. Environmental science &. technology 28, 670–674, https://doi.org/10.1021/es00053a021 (1994).

41. 41.

Dhananjeyan, M. R. et al. Photodynamics and surface characterization of TiO2 and Fe2O3 photocatalysts immobilized on modified polyethylene films. The Journal of Physical Chemistry B 105, 12046–12055, https://doi.org/10.1021/jp011339q (2001).

42. 42.

Uchida, H. et al. Preparation and properties of size-quantized TiO2 particles immobilized in poly(vinylpyrrolidinone) gel films. Langmuir 11, 3725–3729, https://doi.org/10.1021/la00010a023 (1995).

43. 43.

Thiruvenkatachari, R., Ouk Kwon, T. & Shik Moon, I. Application of Slurry Type Photocatalytic Oxidation‐Submerged Hollow Fiber Microfiltration Hybrid System for the Degradation of Bisphenol A (BPA). Separation Science and Technology 40, 2871–2888, https://doi.org/10.1080/01496390500333160 (2005).

44. 44.

Mishra, G. & Mukhopadhyay, M. Flux improvement, rejection, surface energy and antibacterial properties of synthesized TiO2-Mo.HNTs/PVC nanocomposite ultrafiltration membranes. New Journal of Chemistry 41, 15049–15057 (2017).

45. 45.

Damodar, R. A., You, S.-J. & Chou, H.-H. Study the self cleaning, antibacterial and photocatalytic properties of TiO2 entrapped PVDF membranes. Journal of Hazardous Materials 172, 1321–1328, https://doi.org/10.1016/j.jhazmat.2009.07.139 (2009).

46. 46.

Wittmar, A., Vorat, D. & Ulbricht, M. Two step and one step preparation of porous nanocomposite cellulose membranes doped with TiO2. RSC Advances 5, 88070–88078, https://doi.org/10.1039/c5ra16337d (2015).

47. 47.

Zhang, H., Quan, X., Chen, S., Zhao, H. & Zhao, Y. Fabrication of photocatalytic membrane and evaluation its efficiency in removal of organic pollutants from water. Separation and purification technology 50, 147–155, https://doi.org/10.1016/j.seppur.2005.11.018 (2006).

48. 48.

Wang, L., Chen, J., Ge, L., Zhu, Z. & Rudolph, V. Halloysite-nanotube-supported Ru nanoparticles for ammonia catalytic decomposition to produce CO x-free hydrogen. Energy & Fuels 25, 3408–3416 (2011).

49. 49.

Yuan, P. et al. Functionalization of halloysite clay nanotubes by grafting with γ-aminopropyltriethoxysilane. The Journal of Physical Chemistry C 112, 15742–15751 (2008).

50. 50.

Datta, K., Achari, A. & Eswaramoorthy, M. Aminoclay: a functional layered material with multifaceted applications. Journal of Materials Chemistry A 1, 6707–6718 (2013).

51. 51.

Li, C., Fu, L., Ouyang, J. & Yang, H. Enhanced performance and interfacial investigation of mineral-based composite phase change materials for thermal energy storage. Scientific reports 3, 1908 (2013).

52. 52.

Yang, H., Li, M., Fu, L., Tang, A. & Mann, S. Controlled assembly of Sb 2 S 3 nanoparticles on silica/polymer nanotubes: insights into the nature of hybrid interfaces. Scientific reports 3, 1336 (2013).

53. 53.

Zhang, Y., He, X., Ouyang, J. & Yang, H. Palladium nanoparticles deposited on silanized halloysite nanotubes: synthesis, characterization and enhanced catalytic property. Scientific reports 3 (2013).

54. 54.

Zhang, Y. & Yang, H. Halloysite nanotubes coated with magnetic nanoparticles. Applied Clay Science 56, 97–102 (2012).

55. 55.

Wang, L., Chen, J., Ge, L., Rudolph, V. & Zhu, Z. Halloysite nanotube supported Ru nanocatalysts synthesized by the inclusion of preformed Ru nanoparticles for preferential oxidation of CO in H2-rich atmosphere. The Journal of Physical Chemistry C 117, 4141–4151 (2013).

56. 56.

Turhan, Y., Dogan, M. & Alkan, M. Poly (vinyl chloride)/kaolinite nanocomposites: characterization and thermal and optical properties. Industrial & Engineering Chemistry Research 49, 1503–1513 (2010).

57. 57.

Mishra, G. & Mukhopadhyay, M. Enhanced antifouling performance of halloysite nanotubes (HNTs) blended poly(vinyl chloride) (PVC/HNTs) ultrafiltration membranes: For water treatment. Journal of Industrial and Engineering Chemistry 63, 366–379 (2018).

58. 58.

Abdel-Monem, Y. K. Efficient nanophotocatalyt of hydrothermally synthesized Anatase TiO 2 nanoparticles from its analogue metal coordinated precursor. Journal of Materials Science: Materials in Electronics 27, 5723–5728 (2016).

59. 59.

Bumajdad, A., Madkour, M., Abdel-Moneam, Y. & El-Kemary, M. Nanostructured mesoporous Au/TiO2 for photocatalytic degradation of a textile dye: the effect of size similarity of the deposited Au with that of TiO2 pores. Journal of Materials Science 49, 1743–1754 (2014).

60. 60.

Ghanbari, M. et al. Super hydrophilic TiO2/HNT nanocomposites as a new approach for fabrication of high performance thin film nanocomposite membranes for FO application. Desalination 371, 104–114, https://doi.org/10.1016/j.desal.2015.06.007 (2015).

61. 61.

Yao, W. et al. Synthesis and characterization of high efficiency and stable Ag3PO4/TiO2 visible light photocatalyst for the degradation of methylene blue and rhodamine B solutions. Journal of Materials Chemistry 22, 4050–4055, https://doi.org/10.1039/c2jm14410g (2012).

62. 62.

Chen, Y., Zhang, Y., Liu, J., Zhang, H. & Wang, K. Preparation and antibacterial property of polyethersulfone ultrafiltration hybrid membrane containing halloysite nanotubes loaded with copper ions. Chemical Engineering Journal 210, 298–308 (2012).

63. 63.

Yu, Z. et al. Effect of functionalized multi-walled carbon nanotubes on the microstructure and performances of PVDF membranes. RSC Advances 5, 75998–76006 (2015).

64. 64.

Bottino, A., Camera-Roda, G., Capannelli, G. & Munari, S. The formation of microporous polyvinylidene difluoride membranes by phase separation. Journal of Membrane Science 57, 1–20 (1991).

65. 65.

Naik, A. P., Salkar, A. V., Majik, M. S. & Morajkar, P. P. Enhanced photocatalytic degradation of Amaranth dye on mesoporous anatase TiO 2: evidence of C–N, N=N bond cleavage and identification of new intermediates. Photochemical & Photobiological Sciences 14, 1126–1138 (2017).

66. 66.

Lee, S.-Y. & Park, S.-J. TiO2 photocatalyst for water treatment applications. Journal of Industrial and Engineering Chemistry 19, 1761–1769, https://doi.org/10.1016/j.jiec.2013.07.012 (2013).

67. 67.

Huo, P. et al. Photocatalytic degradation of antibiotics in water using metal ion@ TiO2/HNTs under visible light. Desalination and Water Treatment 52, 6985–6995 (2014).

68. 68.

Srivastava, N. & Mukhopadhyay, M. Biosynthesis of SnO2 nanoparticles using bacterium Erwinia herbicola and their photocatalytic activity for degradation of dyes. Industrial & Engineering Chemistry Research 53, 13971–13979 (2014).

69. 69.

Zinadini, S., Zinatizadeh, A. A., Rahimi, M., Vatanpour, V. & Zangeneh, H. Preparation of a novel antifouling mixed matrix PES membrane by embedding graphene oxide nanoplates. Journal of Membrane Science 453, 292–301 (2014).

70. 70.

Gupta, V. K. et al. Photo-catalytic degradation of toxic dye amaranth on TiO2/UV in aqueous suspensions. Materials Science and Engineering: C 32, 12–17 (2012).

71. 71.

Daneshvar, N., Salari, D. & Khataee, A. Photocatalytic degradation of azo dye acid red 14 in water on ZnO as an alternative catalyst to TiO2. Journal of photochemistry and photobiology A: chemistry 162, 317–322 (2004).

72. 72.

Chakrabarti, S. & Dutta, B. K. Photocatalytic degradation of model textile dyes in wastewater using ZnO as semiconductor catalyst. Journal of Hazardous Materials 112, 269–278 (2004).

73. 73.

Sharma, S., Mukhopadhyay, M. & Murthy, Z. Rate parameter estimation for 4-chlorophenol degradation by UV and organic oxidants. Journal of Industrial and Engineering Chemistry 18, 249–254 (2012).

74. 74.

Abdel-Monem, Y. K., Emam, S. M. & Okda, H. M. Solid state thermal decomposition synthesis of CuO nanoparticles from coordinated pyrazolopyridine as novel precursors. Journal of Materials Science: Materials in Electronics 28, 2923–2934 (2017).

75. 75.

Zhao, Y., Abdullayev, E., Vasiliev, A. & Lvov, Y. Halloysite nanotubule clay for efficient water purification. Journal of Colloid and Interface Science 406, 121–129 (2013).

76. 76.

Mansourpanah, Y., Madaeni, S., Rahimpour, A., Farhadian, A. & Taheri, A. Formation of appropriate sites on nanofiltration membrane surface for binding TiO 2 photo-catalyst: performance, characterization and fouling-resistant capability. Journal of Membrane Science 330, 297–306 (2009).

77. 77.

Madaeni, S. & Ghaemi, N. Characterization of self-cleaning RO membranes coated with TiO2 particles under UV irradiation. Journal of Membrane Science 303, 221–233 (2007).

78. 78.

Lawless, D., Serpone, N. & Meisel, D. Role of hydroxyl radicals and trapped holes in photocatalysis. A pulse radiolysis study. The Journal of Physical Chemistry 95, 5166–5170, https://doi.org/10.1021/j100166a047 (1991).

79. 79.

Houas, A. et al. Photocatalytic degradation pathway of methylene blue in water. Applied Catalysis B: Environmental 31, 145–157, https://doi.org/10.1016/S0926-3373(00)00276-9 (2001).

80. 80.

Jo, W.-K. & Tayade, R. J. Recent developments in photocatalytic dye degradation upon irradiation with energy-efficient light emitting diodes. Chinese Journal of Catalysis 35, 1781–1792, https://doi.org/10.1016/S1872-2067(14)60205-9 (2014).

81. 81.

Jing, H.-P., Wang, C.-C., Zhang, Y.-W., Wang, P. & Li, R. Photocatalytic degradation of methylene blue in ZIF-8. RSC Advances 4, 54454–54462 (2014).

82. 82.

Yogi, C. et al. Photocatalytic degradation of methylene blue by TiO2 film and Au particles-TiO2 composite film. Thin Solid Films 516, 5881–5884 (2008).

83. 83.

Orendorz, A., Ziegler, C. & Gnaser, H. Photocatalytic decomposition of methylene blue and 4-chlorophenol on nanocrystalline TiO2 films under UV illumination: A ToF-SIMS study. Applied surface science 255, 1011–1014 (2008).

84. 84.

Rauf, M. A., Meetani, M. A., Khaleel, A. & Ahmed, A. Photocatalytic degradation of Methylene Blue using a mixed catalyst and product analysis by LC/MS. Chemical Engineering Journal 157, 373–378 (2010).

85. 85.

Fischer, K. et al. Photoactive microfiltration membranes via directed synthesis of TiO2 nanoparticles on the polymer surface for removal of drugs from water. Journal of Membrane Science 478, 49–57 (2015).

86. 86.

Sugimoto, T., Zhou, X. & Muramatsu, A. Synthesis of uniform anatase TiO2 nanoparticles by gel–sol method: 3. Formation process and size control. Journal of colloid and interface science 259, 43–52 (2003).

87. 87.

Hassanien, A. S. & Akl, A. A. Influence of composition on optical and dispersion parameters of thermally evaporated non-crystalline Cd50S50−xSex thin films. Journal of Alloys and Compounds 648, 280–290, https://doi.org/10.1016/j.jallcom.2015.06.231 (2015).

88. 88.

Madkour, M., Abdel-Monem, Y. K. & Al Sagheer, F. Controlled synthesis of NiO and Co3O4 nanoparticles from different coordinated precursors: impact of precursor’s geometry on the nanoparticles characteristics. Industrial & Engineering Chemistry Research 55, 12733–12741 (2016).

89. 89.

Liu, P., Liu, H., Liu, G., Yao, K. & Lv, W. Preparation of TiO2 nanotubes coated on polyurethane and study of their photocatalytic activity. Applied surface science 258, 9593–9598, https://doi.org/10.1016/j.apsusc.2012.05.154 (2012).

90. 90.

You, S.-J., Semblante, G. U., Lu, S.-C., Damodar, R. A. & Wei, T.-C. Evaluation of the antifouling and photocatalytic properties of poly(vinylidene fluoride) plasma-grafted poly(acrylic acid) membrane with self-assembled TiO2. Journal of Hazardous Materials 237-238, 10–19, https://doi.org/10.1016/j.jhazmat.2012.07.071 (2012).

91. 91.

Alem, A., Sarpoolaky, H. & Keshmiri, M. Titania ultrafiltration membrane: Preparation, characterization and photocatalytic activity. Journal of the European Ceramic Society 29, 629–635, https://doi.org/10.1016/j.jeurceramsoc.2008.07.003 (2009).

## Acknowledgements

Authors express sincere gratitude to the Sophisticated Analytical Instrument Facility (SAIF), Metallurgical Engineering and Materials Science (MEMS) Indian Institute of Technology Bombay (IIT-B), CSIR-National Chemical Laboratory (CSIR-NCL) Pune and Indian Institute of Technology Gandhi Nagar (IIT-GN) for providing characterization facilities. We are also thankful to the Department of Chemical Engineering, SVNIT, Surat for providing research facilities and MHRD Govt. of India for providing fellowship.

## Author information

Authors

### Contributions

Mausumi Mukhopadhyay conceptualized the research work and supervised the work done all through with details contribution in discussing and reviewing of the manuscript with technical inputs. Gourav Mishra as part of his PhD research performed all the experiments, characterization, and test, calculation, drawn Figure 13, and data analysis of all results and wrote the manuscript.

## Ethics declarations

### Competing Interests

The authors declare no competing interests.

Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Mishra, G., Mukhopadhyay, M. TiO2 decorated functionalized halloysite nanotubes (TiO2@HNTs) and photocatalytic PVC membranes synthesis, characterization and its application in water treatment. Sci Rep 9, 4345 (2019). https://doi.org/10.1038/s41598-019-40775-4

• Accepted:

• Published:

• ### Surface-Modified Halloysite Nanotubes as Electrochemical CO2 Sensors

• Kannika Jeamjumnunja
• , Orrapa Cheycharoen
• , Nattida Phongzitthiganna
• , Supa Hannongbua
•  & Chaiya Prasittichai

ACS Applied Nano Materials (2021)

• ### TiO2@HNTs Robustly Decorated PVDF Membrane Prepared by a Bioinspired Accurate-Deposition Strategy for Complex Corrosive Wastewater Treatment

• Jingcheng Wu
• , Yi He
• , Liang Zhou
• , Xiangying Yin
• , Liyun Zhang
• , Jingyu Chen
• , Zhenyu Li
•  & Yang Bai

ACS Applied Materials & Interfaces (2021)

• ### Photocatalytic Oxidation of PLA/TiO2-Composite Films for Indoor Air Purification

• Pattamaphon Chanklom
• , Torpong Kreetachat
• , Rotruedee Chotigawin
•  & Kowit Suwannahong

ACS Omega (2021)

• ### NiS/Pt nanoparticles co-decorated black mesoporous TiO2 hollow nanotube assemblies as efficient hydrogen evolution photocatalysts

• Shijie Wang
• , Huapeng Sun
• , Panzhe Qiao
• , Zhenzi Li
• , Ying Xie
•  & Wei Zhou

Applied Materials Today (2021)

• ### Well dispersed CeO2@HNTs nanofiller in the poly (vinyl chloride) membrane matrix and enhanced its antifouling properties and rejection performance

• Gourav Mishra

Journal of Environmental Chemical Engineering (2021)